Thank you for visiting nature.com. You are using a browser version with limited support for CSS. To obtain the best experience, we recommend you use a more up to date browser (or turn off compatibility mode in Internet Explorer). In the meantime, to ensure continued support, we are displaying the site without styles and JavaScript.

Sign changing pairing in single layer FeSe/SrTiO3 revealed by nonmagnetic impurity bound states

Abstract

The discovery of high-temperature superconductivity in single layer FeSe epitaxially grown on SrTiO3(001) substrates has instigated extensive debate over whether its pairing symmetry is conventional sign-preserving s-wave or unconventional sign-changing. Here, we probe the pairing state for single layer FeSe/SrTiO3 grown by molecular beam epitaxy using scanning tunneling microscopy/spectroscopy. We observe robust in-gap bound states induced by non-magnetic Fe-vacancy defects within the Fe-plane, which exhibit strong spatial electron-hole asymmetry with two-fold symmetry in hole states and four-fold in electron states. The bound states exhibit no energy shift or splitting under an applied magnetic field, consistent with a sign-changing order parameter. This is further confirmed by defect bound state quasiparticle interference that shows a sign-changing behavior with a pair of corresponding peaks at the positive and negative energies near the impurity bound states. Our findings provide unambiguous evidence for a sign-changing pairing symmetry for single layer FeSe/SrTiO3.

Introduction

The Cooper pairs in a superconductor can be locally broken by impurity scattering, leading to Bogoliubov quasiparticle excitations that can reveal the nature of the superconducting pairing state1. For conventional superconductors, only magnetic impurities can break the Cooper pairs, while for unconventional superconductors, both magnetic and non-magnetic impurities can induce such bound states. Hence, probing bound states and quasi-particle scattering at the atomic scale using scanning tunneling microscopy/spectroscopy (STM/S) has been a proven phase-sensitive method for probing pairing symmetry of superconductors. Well known examples include the observation of asymmetric spatial distribution of bound states for electrons and holes in cuprates, which provides unambiguous evidence for dx2–y2 wave pairing1,2,3,4.

For Fe based superconductors, the determination of pairing symmetry has been challenging due to the multiple bands crossing the Fermi level, giving rise to a number of pairing symmetries5. The recent discovery of high-temperature superconductivity in single-layer FeSe epitaxially grown on SrTiO3(001) substrate6,7 provides a model system to probe the pairing states of Fe-based superconductors. Because of electron doping from the STO substrate8, the Fermi surface of FeSe/STO consists of only electron pockets at the Brillouin zone (BZ) corner M points, while the hole pockets at Γ point are entirely below the Fermi energy9,10. The lack of hole pockets challenges the spin fluctuation picture that involves a sign reversal order parameter between the electron and hole pockets11,12. This has instigated extensive debate on the symmetry of pairing state in single-layer FeSe, with leading contender being sign-preserving conventional s-wave pairing13, and unconventional sign-changing extended s-wave14,15 and nodeless d-wave pairing16,17,18,19, hence experimental validation are sorely needed20.

Impurity scattering has been utilized to investigate the superconducting pairing symmetry of single-layer FeSe/STO, however with conflicting results13,21,22. A plain s-wave has been suggested in an earlier STM work13, based on quasiparticle interference off adsorbates on the surface of FeSe, where no impurity-induced bound states were observed for nonmagnetic Zn, Ag, and K adatoms. However, more recent work shows that even for nonmagnetic surface K21 and Pb adatoms22, bound states near the superconducting gap edge were found after careful data analysis. The emergence of the induced bound states by these nonmagnetic surface adatoms21,22 indicates sign-reversing pairing scenarios, challenging the plain s-wave pairing symmetry. One concern for scattering by surface adatoms is that the induced bound states are located near the superconducting gap edges due to weak scattering23, which may be challenging to discern due to their close proximity to the coherence peaks. As such, the pairing symmetry for single-layer FeSe/STO remains controversial, and unambiguous verification of induced in-gap bound states and quasiparticle scattering off nonmagnetic impurities within the Fe plane is crucial.

In this work, we probe bound states induced by non-magnetic impurities within the Fe-plane of single-layer FeSe/STO, whose nonmagnetic nature is verified by magnetic field dependent studies. We observe robust in-gap bound states with strong spatial electron-hole asymmetry, which provides clear evidence for sign-changing pairing symmetry. We further carry out systematic impurity scattering studies and apply the recently proposed defect bound state (DBS) quasiparticle interference (QPI) method24,25,26,27 to provide additional support for a sign reversal pairing order parameter, consistent with extended s-wave14,15 or nodeless d-wave pairing16.

Results

Non-magnetic defects in single-layer FeSe/STO

Figure 1a shows typical surface morphology of superconducting single-layer FeSe film that is conformal to the step-terrace morphology of the STO substrate. The film is also characterized by a high density of grain boundaries (GBs), appearing as a network of meandering lines with low contrast, similar to previous reports6,7. dI/dV spectroscopy reveals a typical “U” shape superconducting gap structure with two coherence peaks, which exhibit spatial variations (Supplementary Fig. 1). Fitting the histogram of the superconducting gaps by Gaussian functions yields an average value of Δ1 = 11.1 ± 0.1 meV and Δ2 = 17.5 ± 0.1 meV, comparable to previous reports6,13,21. The superconducting transition temperature (TC) is 60 K from our own angle resolved photoemission spectroscopy (ARPES) measurements28, comparable to 65 K in previous reports10.

While defect density on as-grown single-layer FeSe/STO film is low, at 5.0 × 1011 cm−2, higher density (1.5 × 1013 cm−2) can be introduced by capping the FeSe films with amorphous Se film first, and then annealing to remove the Se layer (Fig. 1b and Supplementary Fig. 2). Five types of defects can be created that are either two- or four-fold symmetric (Supplementary Fig. 3). Accounting for 90% of all defects are of types A and B (Fig. 1c, d), which are centered at the bridge site, i.e., Fe site, of the top-layer Se lattice, and appear as a dumbbell consisting of two bright lobes that are asymmetric in intensity at adjacent Se sites29,30. These dumbbell features have been reported in earlier studies and attributed to Fe vacancy and SeFe substitutional defects. While the nature of the dumbbell defects is still under debate21,29, comparison between our density functional theory calculations and STM images taken at liquid nitrogen temperature indicates that type A defects are Fe vacancies (Supplementary Fig. 4). In contrast, the four-fold symmetric defects (Supplementary Fig. 3c–e) are located at Se sites, likely Se-site related defects21, and therefore are not the focus of this work.

dI/dV spectra taken at the center of dumbbell defects show strongly suppressed coherence peaks as well as pronounced resonance peaks inside the superconducting gap, as depicted in Fig. 1e, f. The energy position of bound states for Type A and B defects are −2.7 meV (inside the superconducting gap) and −8.3 meV (near the inner coherence peak), respectively. The resonance peak at the center of the impurity site can be up to three times stronger than the normal state conductance. Magnetic field dependent measurements (Fig. 1e, f) further indicate that while the intensities of these states are slightly suppressed in an external magnetic field; no shift or splitting of these peaks are observed up to 9 T out-of-plane or 2 T in-plane fields, indicating both these types of defects are nonmagnetic.

We have also carried out tunneling spectroscopy measurements at 400 mK with improved energy resolution of 0.36 meV, as determined by measuring the superconducting gap of a well-known superconductor Pb (Supplementary Fig. 5), which should be sufficient to resolve the 1 meV Zeeman splitting that’s typical for this material system31. Magnetic-field dependent dI/dV spectra of the dumbbell defects taken at this temperature are shown in Supplementary Fig. 6, where again no shifting or splitting of the bound states are observed at ±9 T magnetic field. Note that while some fluctuations in the energy position of the bound state are observed with magnetic field, they are within the spectral energy resolution, and do not show a linear dependence on the magnetic field as would be expected from Zeeman effect. These results unambiguously indicate that the dumbbell defects, both type A and type B, are not magnetic.

We further note that these observations are in marked contrast to magnetic Fe vacancy defects in KFe2Se2 films31, where an energy shift of 1 meV (at 9 T) is resolved at 400 mK, as well as a clear linear magnetic field dependence of the energy position of the bound states.

Spatial and energy dependence of bound states

Differential conductance maps of Type A dumbbell defect (Fig. 2a) further reveal that these in-gap bound states are confined to the vicinity of the defects in real space, but do exhibit a different spatial distribution for the electron- and hole-like states. Specifically, the hole-like bound state at −4.4 meV exhibits a two-fold symmetry (Fig. 2b), while the electron-like bound state at +4.4 meV exhibits a four-fold symmetry (Fig. 2c) as schematically shown in Fig. 2d. The intensity for the hole-like bound state is the strongest directly at the impurity site (Fig. 2e). In contrast, the electron-like bound state has the highest intensity at the four lobes, as shown in the dI/dV spectrum taken at one of the lobes (Fig. 2f). A strong electron-hole asymmetry is clearly seen here where the local maxima and minima occur at different lattice sites with respect to the impurity. A detailed site dependent measurement of the bound states is shown in Supplementary Fig. 7, where the intensity of the hole state decreases from the defect site to the nearest neighbor (NN), next nearest neighbor (NNN), 3rd NN, and so on, while the electron state emerges, with increasing intensity in the reverse order, reaching maximum at 3rd NN. Overall, the spatial distribution at +4.4 meV shows a C2 symmetry, while at −4.4 meV it is approximately C4 symmetric. Moreover, the C2 symmetry is along the dumbbell defect direction (Fig. 2b), whereas the relatively bright four-fold region is along the Fe–Fe direction (Fig. 2c), 45° to the Se–Se lattice, consistent with the C4 symmetry of the superconducting Fe plane. Similar electron-hole asymmetry is also observed for type B defect, as shown in Supplementary Fig. 8. These observations of the in-gap bound states and spatial electron-hole asymmetry are similar to those of d-wave cuprate superconductors1,2,3, indicating an unconventional pairing symmetry in single-layer FeSe/STO. Note that measurements at 77 K indicate that there are no impurity states within ±45 meV of the Fermi level for type A defects (Supplementary Fig. 9b). Furthermore, dI/dV maps between ±20 meV exhibit no electron-hole asymmetry (Supplementary Fig. 9c–n) in the normal state.

The presence of these defects, however, modifies the normal states around −0.26 eV. For type A, the peak shifts towards the Fermi level by as much as 14 meV (Supplementary Fig. 10b), indicating local hole doping. In contrast, for type B defects, the peak moves away from the Fermi level (Supplementary Fig. 10d), consistent with electron doping8,32. Interestingly, these shifts in the normal states are also directly correlated with the energy positions of the bound states. For example, for the three type A defects I, II, and III (marked in Figs. 1b and 3a–c), the bound states shift towards the Fermi level in tandem with the normal state as shown in Fig. 3d, e. Analysis of up to 70 defects indicates that the bound state energy position can vary between −1.7 and −7.5 meV. Plotted in Fig. 3f, g are histogram of the bound states, and the correlation between the normal-state and the bound-state peak energies. While the origin of such correlation is not known at the moment, the normal-state peak energy shifts downward as the bound state shifts towards the superconducting edge, suggesting that local electron doping is one of the possible causes for the energy shift of the bound states. Note that this behavior deviates from that of LiFeAs, where the bound states induced by different impurities are pinned near the coherence peaks33.

These observations of in-gap bound states induced by non-magnetic impurities within the Fe plane, particularly their spatial electron-hole asymmetry, i.e., a two-fold hole-like state and four-fold electron-like state, are the defining signatures of Bogoliubov quasiparticle excitations. In turn they strongly suggest a sign-changing unconventional order parameter in single-layer FeSe/STO, which is further confirmed by the defect bound state phase-referenced QPI discussed below.

Defect bound state phase-referenced quasiparticle interference

Impurities, particularly those located within the Fe plane such as Fe vacancies can serve as strong scattering centers for quasiparticles and produce standing waves in real space (Fig. 4a), which can be better seen in the energy dependent conductance maps in Fig. 4b–d. Fast Fourier transforms (FFTs) of these conductance maps reveal information in the momentum space that can be understood by comparing to Fermi surface maps obtained from ARPES9,10, also sketched here in Fig. 4e. Results for three representative energies are shown in Fig. 4f–h, with additional data at other energies between ±20 meV presented in Supplementary Figs. 11 and 12. The FFTs are four-fold symmetrized and subtracted by a 2D-gaussian-function background around Γ point to improve signal-to-noise ratio. Similar to previous reports13,34, typical nine-ring features in q space are observed, produced by quasiparticle scattering including intra-pocket q1 and inter-pocket q2 and q3 as labeled in Fig. 4f. The scattering rings induced by q2 and q3 appear more as arcs, lacking four-fold symmetry, likely related to orbital features13.

While these FFTs yield the intensities of scattering channels, they do not provide any phase information. For unconventional superconductors with sign change between different Fermi surfaces, additional phase shifts are expected near the bound state induced by nonmagnetic impurities. This phase information can be obtained from the recently developed defect bound states-QPI technique24,25,26,27, where a pair of positive and negative peaks are expected to appear in gpr (q, +E) and gpr (q, −E), respectively, at energies near the nonmagnetic impurity bound-state energies ±EB (see Methods).

For a type A defect (located at the center of the maps), a series of phase-referenced QPI gpr(q, E) are calculated following Eqs. (1)–(3) (see Methods). Results at ±4.4 meV (bound state energy) and ±10.4 meV (coherence peak of Δ1) are shown in Fig. 5a–h, with additional data at other energies between ±12 meV presented in Supplementary Figs. 13 and 14. For positive energies (Fig. 5e, f), gpr(q, E) are positive everywhere, as expected. On the other hand, at negative energies (Fig. 5g, h), both positive and negative values are observed. Particularly for E = −4.4 meV, the region between the two circles (defined by 0.24π/a < q < 0.64π/a, where a is the Fe–Fe bond length) is overwhelmingly negative, indicating that this pocket contains a sign-reversal inter- or intra-pocket scattering. The extent of this region changes with energy, which can be better illustrated by integrating the signal within the area as a function of energy, as shown in Fig. 5i. Clearly, a positive and negative peak is seen at + and − 4.4 meV, respectively, which are energy positions of the impurity-induced bound states, indicating a sign changing pairing parameter for single-layer FeSe/STO. We note that this defect bound states-QPI method was also applied to (Li1−xFex)OHFe1−yZnySe, where a similar conclusion on sign-changing pairing was drawn26.

The selection of the integrated range is based on the following considerations. First, signals at small q are not included as they are usually due to disorder. Second, the integrated regions are carefully determined based on the topography of the Fermi surface. As it is difficult to distinguish q1 from different scattering channels, the area is selected so that the total signal due to inter- and intra-band large q-scattering are all well covered. The integral region is selected as 0.24/aSe < q < 0.64/aSe, slight smaller than that of (Li1−xFex)OHFe1−yZnySe (0.18/aSe < q < 0.77/aSe35 or 0.37/aSe < q < 0.74/aSe26), due to the smaller electron pockets at M point for single-layer FeSe/STO36. Calculations were done for three different integrated areas: 0.24π/a < q < 0.64π/a, 0.32π/a < q < 0.64π/a, and 0.24π/a < q < 0.72π/a, where similar positive and negative peaks are observed at the in-gap bound state energy, only with slight differences in intensity (Supplementary Fig. 15), further demonstrating that the appearances of these peaks are not due to artifacts such as integration areas.

Similar analysis was done for another type A defect with bound states located at ±6.4 meV (Supplementary Fig. 16), as well as a type B defect with bound states at ±9.0 meV (Supplementary Fig. 17), where corresponding positive and negative peaks were also observed, further supporting sign-changing scenarios.

Discussion

Single-layer FeSe/STO only consists of electron pockets at M point and meanwhile, it is fully gapped without nodes. Therefore, the three possible pairing symmetries are plain s-wave, nodeless d-wave, and bonding-antibonding s-wave20, as summarized in Supplementary Fig. 18. A plain s-wave has been suggested13 based on quasiparticle interference off adsorbates on the surface of FeSe, where impurity-induced bound states were observed only for magnetic impurities. However, recent work clearly shows that even nonmagnetic surface adsorbates such as K and Pb can induce bound states near the superconducting gap edge21,22, indicating sign-reversing pairing scenarios. In this work, in-gap bound states from a nonmagnetic impurity within the Fe plane is observed, which exhibit a strong spatial electron-hole asymmetry, also indicating a sign-changing pairing parameter. This is further confirmed by our phase-referenced defect bound state QPI data. Thus, the possibility of plain s-wave can be ruled out, which leaves two scenarios for the pairing symmetry of single-layer FeSe/STO: s+− and nodeless d-wave. However, in both cases, scattering between Fermi surfaces of different orbital character with different signs are possible (Supplementary Fig. 19), and hence cannot be distinguished by this method. Our recent work shows that one-dimensional scattering where the momentum q is always perpendicular to edges can provide a means to further differentiate these two pairing scenarios37.

In conclusion, we systematically studied the in-gap bound states induced by nonmagnetic impurities within the Fe-plane in single-layer FeSe/STO by STM/S. These bound states exhibit a strong spatial electron-hole asymmetry whose energy position is correlated with local doping. We further carried out phase-referenced defect bound state QPI, which reveals corresponding positive and negative peaks at the bound state energies, indicating a sign change for the order parameter. Our findings provide critical insight into the pairing symmetry of this intriguing high temperature superconductor single-layer FeSe/STO.

Methods

MBE growth and STM/S characterization

Single layer FeSe films were prepared by MBE under Se-rich conditions using high purity Fe (99.995%) and Se (99.9999%) from an e-beam source and a K-cell on the Nb-doped (0.05 wt.%) SrTiO3(001) substrate at 400 °C. The as-grown FeSe films were capped with 20 nm amorphous Se films, and then transferred in air to a Unisoku-1300 STM system (air exposure time < 15 min), where they were annealed first at 200 °C for 2 h to remove the extra Se and subsequently at between 460 and 480 °C for 1 h to reach superconductivity. Low-temperature STM/S measurements were carried out using a polycrystalline PtIr tip. The STS was acquired by using a lock-in technique with a bias modulation Vrms = 0.5 mV at 732 Hz, unless otherwise specified.

Defect bound state QPI24,25,26,27

For E > 0, the phase-referenced QPI signals gpr(q, E) are expressed as

$$g_{pr}\left( {{\mathbf{q}},\, + E} \right) = \left| {g\left( {{\mathbf{q}},\, + E} \right)} \right| \times Re\left[ {e^{i\left( {\theta _{{\mathbf{q}},\, + E} - \theta _{{\mathbf{q}},\, + E}} \right)}} \right] = \left| {g\left( {{\mathbf{q}},\, + E} \right)} \right|$$
(1)
$$g_{pr}\left( {{\mathbf{q}},\, - E} \right) = \left| {g\left( {{\mathbf{q}},\,- E} \right)} \right| \times Re\left[ {e^{i\left( {\theta _{{\mathbf{q}},\,\,- E} - \theta _{{\mathbf{q}},\, + E}} \right)}} \right] = \left| {g\left( {{\mathbf{q}},\, - E} \right)} \right|\cos \left( {\theta _{{\mathbf{q}},\, - E} - \theta _{{\mathbf{q}},\, + E}} \right)$$
(2)

The phase term can be expressed as

$$\cos \left( {\theta _{{\mathbf{q}},\, - E} - \theta _{{\mathbf{q}},\, + E}} \right) = \cos \theta _{{\mathbf{q}},\, - E}\cos \theta _{{\mathbf{q}},\, + E} + \sin \theta _{{\mathbf{q}},\, - E}\sin \theta _{{\mathbf{q}},\, + E}\\ = \frac{{Re[g({\mathbf{q}},\, - E)]}}{{\left| {g({\mathbf{q}},\, - E)} \right|}}\frac{{Re[g({\mathbf{q}},\, + E)]}}{{\left| {g({\mathbf{q}},\, + E)} \right|}} + \frac{{Im[g({\mathbf{q}},\, - E)]}}{{\left| {g({\mathbf{q}},\, - E)} \right|}}\frac{{Im[g({\mathbf{q}},\, + E)]}}{{\left| {g({\mathbf{q}},\, + E)} \right|}}$$
(3)

Here, Re denotes the real part of $$g({\mathbf{q}},E)$$ while Im denotes the imaginary part. Based on Eq. (1), $$g_{pr}\left( {{\mathbf{q}},\,+E} \right)$$ is always positive at positive energy, while at negative energy $$g_{pr}\left( {{\mathbf{q}}, \,- E} \right)$$ is determined by the phase term $$\cos ( {\theta _{{\mathbf{q}},\, - E} - \theta _{{\mathbf{q}},\, + E}} )$$. If there is a sign change between the initial and final state, the phase shift would be π, hence inducing a negative value since $$\cos ( {\theta _{{\mathbf{q}},\, - E} - \theta _{{\mathbf{q}},\, + E}} )$$=$$\cos \left( \pi \right)$$= −1.

Data availability

The data supporting the findings of this study are available within the paper, its Supplementary Information files, and from the corresponding author upon reasonable request.

References

1. 1.

Balatsky, A. V., Vekhter, I. & Zhu, J.-X. Impurity-induced states in conventional and unconventional superconductors. Rev. Mod. Phys. 78, 373–433 (2006).

2. 2.

Pan, S. H. et al. Imaging the effects of individual zinc impurity atoms on superconductivity in Bi2Sr2CaCu2O8+δ. Nature 403, 746–750 (2000).

3. 3.

Hudson, E. W. et al. Interplay of magnetism and high-Tc superconductivity at individual Ni impurity atoms in Bi2Sr2CaCu2O8+δ. Nature 411, 920 (2001).

4. 4.

Choubey, P., Kreisel, A., Berlijn, T., Andersen, B. M. & Hirschfeld, P. J. Universality of scanning tunneling microscopy in cuprate superconductors. Phys. Rev. B 96, 174523 (2017).

5. 5.

Hirschfeld, P. J. Using gap symmetry and structure to reveal the pairing mechanism in Fe-based superconductors. Comptes Rendus Phys. 17, 197–231 (2016).

6. 6.

Qing-Yan, W. et al. Interface-induced high-temperature superconductivity in single unit-cell FeSe films on SrTiO3. Chin. Phys. Lett. 29, 037402 (2012).

7. 7.

Zhang, W.-H. et al. Direct observation of high-temperature superconductivity in one-unit-cell FeSe films. Chin. Phys. Lett. 31, 017401 (2014).

8. 8.

Zhang, H. et al. Origin of charge transfer and enhanced electron–phonon coupling in single unit-cell FeSe films on SrTiO3. Nat. Commun. 8, 214 (2017).

9. 9.

Liu, D. et al. Electronic origin of high-temperature superconductivity in single-layer FeSe superconductor. Nat. Commun. 3, 931 (2012).

10. 10.

He, S. et al. Phase diagram and electronic indication of high-temperature superconductivity at 65 K in single-layer FeSe films. Nat. Mater. 12, 605–610 (2013).

11. 11.

Mazin, I. I., Singh, D. J., Johannes, M. D. & Du, M. H. Unconventional superconductivity with a sign reversal in the order parameter of LaFeAsO1-xFx. Phys. Rev. Lett. 101, 057003 (2008).

12. 12.

Kuroki, K. et al. Unconventional pairing originating from the disconnected Fermi surfaces of superconducting LaFeAsO1-xFx. Phys. Rev. Lett. 101, 087004 (2008).

13. 13.

Fan, Q. et al. Plain s-wave superconductivity in single-layer FeSe on SrTiO3 probed by scanning tunnelling microscopy. Nat. Phys. 11, 946–952 (2015).

14. 14.

Mazin, I. I. Symmetry analysis of possible superconducting states in KxFeySe2 superconductors. Phys. Rev. B 84, 024529 (2011).

15. 15.

Khodas, M. & Chubukov, A. V. Interpocket pairing and gap symmetry in Fe-based superconductors with only electron pockets. Phys. Rev. Lett. 108, 247003 (2012).

16. 16.

Agterberg, D. F., Shishidou, T., O’Halloran, J., Brydon, P. M. R. & Weinert, M. Resilient nodeless d-wave superconductivity in monolayer FeSe. Phys. Rev. Lett. 119, 267001 (2017).

17. 17.

Maier, T. A., Graser, S., Hirschfeld, P. J. & Scalapino, D. J. d-wave pairing from spin fluctuations in the KxFe2-ySe2 superconductors. Phys. Rev. B 83, 100515 (2011).

18. 18.

Wang, F. et al. The electron pairing of KxFe2−ySe2. EPL Europhys. Lett. 93, 57003 (2011).

19. 19.

Kreisel, A. et al. Orbital selective pairing and gap structures of iron-based superconductors. Phys. Rev. B 95, 174504 (2017).

20. 20.

Huang, D. & Hoffman, J. E. Monolayer FeSe on SrTiO3. Annu. Rev. Condens. Matter Phys. 8, 311–336 (2017).

21. 21.

Liu, C. et al. Extensive impurity-scattering study on the pairing symmetry of monolayer FeSe films on SrTiO3. Phys. Rev. B 97, 024502 (2018).

22. 22.

Liu, C. et al. Spectroscopic imaging of quasiparticle bound states induced by strong nonmagnetic scatterings in one-unit-cell FeSe/SrTiO3. Phys. Rev. Lett. 123, 036801 (2019).

23. 23.

Chen, X., Mishra, V., Maiti, S. & Hirschfeld, P. J. Effect of nonmagnetic impurities on s± superconductivity in the presence of incipient bands. Phys. Rev. B 94, 054524 (2016).

24. 24.

Chi, S. et al. Determination of the superconducting order parameter from defect bound state quasiparticle interference. Preprint at https://arxiv.org/abs/1710.09089 (2017).

25. 25.

Chi, S. et al. Extracting phase information about the superconducting order parameter from defect bound states. Preprint at https://arxiv.org/abs/1710.09088 (2017).

26. 26.

Gu, Q. et al. Sign-reversal superconducting gaps revealed by phase-referenced quasiparticle interference of impurity-induced bound states in Li1-xFexOHFe1-yZnySe. Phys. Rev. B 98, 134503 (2018).

27. 27.

Chen, M. et al. Direct visualization of sign-reversal s± superconducting gaps in FeTe0.55Se0.45. Phys. Rev. B 99, 014507 (2019).

28. 28.

Yang, M., Yan, C., Ma, Y., Li, L. & Cen, C. Light induced non-volatile switching of superconductivity in single layer FeSe on SrTiO3 substrate. Nat. Commun. 10, 1–7 (2019).

29. 29.

Huang, D. et al. Dumbbell defects in FeSe films: A scanning tunneling microscopy and first-principles investigation. Nano Lett. 16, 4224–4229 (2016).

30. 30.

Choubey, P., Berlijn, T., Kreisel, A., Cao, C. & Hirschfeld, P. J. Visualization of atomic-scale phenomena in superconductors: application to FeSe. Phys. Rev. B 90, 134520 (2014).

31. 31.

Li, W. et al. Phase separation and magnetic order in K-doped iron selenide superconductor. Nat. Phys. 8, 126–130 (2012).

32. 32.

Tang, C. et al. Superconductivity dichotomy in K-coated single and double unit cell FeSe films on SrTiO3. Phys. Rev. B 92, 180507 (2015).

33. 33.

Chi, S. et al. Impact of iron-site defects on superconductivity in LiFeAs. Phys. Rev. B 94, 134515 (2016).

34. 34.

Huang, D. et al. Revealing the empty-state electronic structure of single-unit-cell FeSe/SrTiO3. Phys. Rev. Lett. 115, 017002 (2015).

35. 35.

Du, Z. et al. Sign reversal of the order parameter in (Li1−xFex)OHFe1−yZnySe. Nat. Phys. 14, 134–139 (2017).

36. 36.

Zhao, L. et al. Common electronic origin of superconductivity in (Li,Fe)OHFeSe bulk superconductor and single-layer FeSe/SrTiO3 films. Nat. Commun. 7, 10608 (2016).

37. 37.

Ge, Z. et al. Evidence for d-wave superconductivity in single layer FeSe/SrTiO3 probed by quasiparticle scattering off step edges. Nano Lett. 19, 2497–2502 (2019).

Acknowledgements

Research supported by the U.S. Department of Energy, Office of Basic Energy Sciences, Division of Materials Sciences and Engineering under Award DE-SC0017632.

Author information

Authors

Contributions

H.Z. and L.L. conceived the research. Z.G. prepared single-layer FeSe/STO films by MBE. H.Z. carried out the low temperature STM/S measurements. M.W. carried out DFT calculations. H.Z. and L.L. analyzed the data and wrote the paper. All authors discussed the results and commented on the paper.

Corresponding author

Correspondence to Lian Li.

Ethics declarations

Competing interests

The authors declare no competing interests.

Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

Rights and permissions

Reprints and Permissions

Zhang, H., Ge, Z., Weinert, M. et al. Sign changing pairing in single layer FeSe/SrTiO3 revealed by nonmagnetic impurity bound states. Commun Phys 3, 75 (2020). https://doi.org/10.1038/s42005-020-0351-1

• Accepted:

• Published: